# CHAPTER OBJECTIVES Show relationship of stress and strain using experimental methods to determine stress-strain diagram of a specific material Discuss.

## Presentation on theme: "CHAPTER OBJECTIVES Show relationship of stress and strain using experimental methods to determine stress-strain diagram of a specific material Discuss."— Presentation transcript:

CHAPTER OBJECTIVES Show relationship of stress and strain using experimental methods to determine stress-strain diagram of a specific material Discuss the behavior described in the diagram for commonly used engineering materials Discuss the mechanical properties and other test related to the development of mechanics of materials

CHAPTER OUTLINE Tension and Compression Test Stress-Strain Diagram Stress-Strain Behavior of Ductile and Brittle Materials Hooke’s Law Strain Energy Poission’s Ratio Shear Stress-Strain Diagram *Failure of Materials Due to Creep and Fatigue

3.1 TENSION & COMPRESSION TEST
Strength of a material can only be determined by experiment One test used by engineers is the tension or compression test This test is used primarily to determine the relationship between the average normal stress and average normal strain in common engineering materials, such as metals, ceramics, polymers and composites

3.1 TENSION & COMPRESSION TEST
Performing the tension or compression test Specimen of material is made into “standard” shape and size Before testing, 2 small punch marks identified along specimen’s length Measurements are taken of both specimen’s initial x-sectional area A0 and gauge-length distance L0; between the two marks Seat the specimen into a testing machine shown below

3.1 TENSION & COMPRESSION TEST
Performing the tension or compression test Seat the specimen into a testing machine shown below The machine will stretch specimen at slow constant rate until breaking point At frequent intervals during test, data is recorded of the applied load P.

3.1 TENSION & COMPRESSION TEST
Performing the tension or compression test Elongation δ = L − L0 is measured using either a caliper or an extensometer δ is used to calculate the normal strain in the specimen Sometimes, strain can also be read directly using an electrical-resistance strain gauge

3.2 STRESS-STRAIN DIAGRAM
A stress-strain diagram is obtained by plotting the various values of the stress and corresponding strain in the specimen Conventional stress-strain diagram Using recorded data, we can determine nominal or engineering stress by P A0 σ = Assumption: Stress is constant over the x-section and throughout region between gauge points

3.2 STRESS-STRAIN DIAGRAM
Conventional Stress-Strain Diagram Likewise, nominal or engineering strain is found directly from strain gauge reading, or by δ L0  = Assumption: Strain is constant throughout region between gauge points By plotting σ (ordinate) against  (abscissa), we get a conventional stress-strain diagram

3.2 STRESS-STRAIN DIAGRAM
Conventional stress-strain diagram Figure shows the characteristic stress-strain diagram for steel, a commonly used material for structural members and mechanical elements

3.2 STRESS-STRAIN DIAGRAM
Conventional stress-strain diagram Elastic behavior. A straight line Stress is proportional to strain, i.e., linearly elastic Upper stress limit, or proportional limit; σpl If load is removed upon reaching elastic limit, specimen will return to its original shape

3.2 STRESS-STRAIN DIAGRAM
Conventional stress-strain diagram Yielding. Material deforms permanently; yielding; plastic deformation Yield stress, σY Figure 3-4 Once yield point reached, specimen continues to elongate (strain) without any increase in load Note figure not drawn to scale, otherwise induced strains is times larger than in elastic limit Material is referred to as being perfectly plastic

3.2 STRESS-STRAIN DIAGRAM
Conventional stress-strain diagram Strain hardening. Ultimate stress, σu While specimen is elongating, its x-sectional area will decrease Figure 3-4 Decrease in area is fairly uniform over entire gauge length

3.2 STRESS-STRAIN DIAGRAM
Conventional stress-strain diagram Necking. At ultimate stress, x-sectional area begins to decrease in a localized region Figure 3-4 As a result, a constriction or “neck” tends to form in this region as specimen elongates further Specimen finally breaks at fracture stress, σf

3.2 STRESS-STRAIN DIAGRAM
Conventional stress-strain diagram Necking. Specimen finally breaks at fracture stress, σf Figure 3-4

3.2 STRESS-STRAIN DIAGRAM
True stress-strain diagram Instead of using original cross-sectional area and length, we can use the actual cross-sectional area and length at the instant the load is measured Values of stress and strain thus calculated are called true stress and true strain, and a plot of their values is the true stress-strain diagram

3.2 STRESS-STRAIN DIAGRAM
True stress-strain diagram In strain-hardening range, conventional σ- diagram shows specimen supporting decreasing load While true σ- diagram shows material to be sustaining increasing stress

3.2 STRESS-STRAIN DIAGRAM
True stress-strain diagram Although both diagrams are different, most engineering design is done within elastic range provided Material is “stiff,” like most metals Strain to elastic limit remains small Error in using engineering values of σ and  is very small (0.1 %) compared to true values

3.3 STRESS-STRAIN BEHAVIOR OF DUCTILE & BRITTLE MATERIALS
Ductile materials Defined as any material that can be subjected to large strains before it ruptures, e.g., mild steel Such materials are used because it is capable of absorbing shock or energy, and if before becoming overloaded, will exhibit large deformation before failing Ductility of material is to report its percent elongation or percent reduction in area at time of fracture

3.3 STRESS-STRAIN BEHAVIOR OF DUCTILE & BRITTLE MATERIALS
Ductile materials Percent elongation is the specimen’s fracture strain expressed as a percent Percent reduction in area is defined within necking region as Percent elongation = Lf − L0 L0 (100%) Percent reduction in area = A0 − Af A0 (100%)

3.3 STRESS-STRAIN BEHAVIOR OF DUCTILE & BRITTLE MATERIALS
Ductile materials Most metals do not exhibit constant yielding behavior beyond the elastic range, e.g. aluminum It does not have well-defined yield point, thus it is standard practice to define its yield strength using a graphical procedure called the offset method

3.3 STRESS-STRAIN BEHAVIOR OF DUCTILE & BRITTLE MATERIALS
Ductile materials Offset method to determine yield strength Normally, a 0.2 % strain is chosen. From this point on the  axis, a line parallel to initial straight-line portion of stress-strain diagram is drawn. The point where this line intersects the curve defines the yield strength.

3.3 STRESS-STRAIN BEHAVIOR OF DUCTILE & BRITTLE MATERIALS
Material that exhibit little or no yielding before failure are referred to as brittle materials, e.g., gray cast iron Brittle materials do not have a well-defined tensile fracture stress, since appearance of initial cracks in a specimen is quite random

3.3 STRESS-STRAIN BEHAVIOR OF DUCTILE & BRITTLE MATERIALS
Instead, the average fracture stress from a set of observed tests is generally reported

3.4 HOOKE’S LAW Most engineering materials exhibit a linear relationship between stress and strain with the elastic region Discovered by Robert Hooke in 1676 using springs, known as Hooke’s law σ = E E represents the constant of proportionality, also called the modulus of elasticity or Young’s modulus E has units of stress, i.e., pascals, MPa or GPa.

3.4 HOOKE’S LAW As shown above, most grades of steel have same modulus of elasticity, Est = 200 GPa Modulus of elasticity is a mechanical property that indicates the stiffness of a material Materials that are still have large E values, while spongy materials (vulcanized rubber) have low values

3.4 HOOKE’S LAW IMPORTANT Modulus of elasticity E, can be used only if a material has linear-elastic behavior. Also, if stress in material is greater than the proportional limit, the stress-strain diagram ceases to be a straight line and the equation is not valid

3.4 HOOKE’S LAW Strain hardening If a specimen of ductile material (steel) is loaded into the plastic region and then unloaded, elastic strain is recovered as material returns to its equilibrium state However, plastic strain remains, thus material is subjected to a permanent set

3.4 HOOKE’S LAW Strain hardening Specimen loaded beyond yield point A to A’ Inter-atomic forces have to be overcome to elongate specimen elastically, these same forces pull atoms back together when load is removed Since E is the same, slope of line O’A’ is the same as line OA

3.4 HOOKE’S LAW Strain hardening Load reapplied, atoms will be displaced until yielding occurs at or near A’, and stress-strain diagram continues along same path as before New stress-strain diagram has higher yield point (A’), a result of strain-hardening Specimen has a greater elastic region and less ductility

3.4 HOOKE’S LAW Strain hardening As specimen is unloaded and loaded, heat or energy may be lost Colored area between the curves represents lost energy and is called mechanical hysteresis It’s an important consideration when selecting materials to serve as dampers for vibrating structures and equipment

Download ppt "CHAPTER OBJECTIVES Show relationship of stress and strain using experimental methods to determine stress-strain diagram of a specific material Discuss."

Similar presentations